Thank you for visiting nature.com. You are using a browser version with limited support for CSS. To obtain the best experience, we recommend you use a more up to date browser (or turn off compatibility mode in Internet Explorer). In the meantime, to ensure continued support, we are displaying the site without styles and JavaScript.

# Photocatalytic air purification mimicking the self-cleaning process of the atmosphere

### Subjects

Photocatalytic air purification is a promising technology that mimics nature’s photochemical process, but its practical applications are still limited despite considerable research efforts in recent decades. Here, we briefly discuss the progress and challenges associated with this technology.

## Photocatalysis as an eco-friendly method of air cleaning

Air pollution severely endangers human health and the environment and requires highly efficient and viable treatment technologies1. There are various technologies for controlling air pollutants, among which adsorption using activated carbons or highly porous materials is the most commonly practised method. However, the adsorbents need to be frequently replaced, the adsorption efficiency is significantly decreased under humid conditions due to the competing adsorption of water vapor, and the equilibrium adsorption capacity is significantly reduced at low concentrations of air pollutants despite the high surface area of the adsorbents. Other technologies, such as ultraviolet radiation, ionization, and nonthermal plasma decomposition, may generate ozone as a harmful by-product. Thermal-catalytic degradation is effective but energy intensive. Biodegradation usually requires large-scale facilities, and its activity is strongly limited by environmental factors. Considering the above limitations, photocatalytic oxidation (PCO) is proposed as an ideal technology for air purification because it can degrade diverse air pollutants into non-toxic or less harmful forms using solar (or artificial) light under ambient conditions2. The photocatalyst (PC) process (eq 1) has some intrinsic similarity to the self-cleaning mechanism in Earth’s atmosphere (eq 2) in that both are based on indirect (sensitized) photooxidation to generate in situ oxidants (e.g., •OH) in air.

$${\mathrm{PC}}\,({\mathrm{heterogeneous}}\,{\mathrm{sensitizer}}\,{\mathrm{such}}\,{\mathrm{as}}\,{\mathrm{Ti}}{{\mathrm{O}}}_{2})+{{\rm{H}}}_{2}{\rm{O}}(g)+h\nu\,\,{\to }\,\,{\scriptstyle{\bullet}} {\rm{OH}}$$
(1)
$${\rm{O}}_{3}({{\mathrm{molecular}}\,{\mathrm{sensitizer}}})+{{\rm{H}}}_{2}{\rm{O}}(g)+h\nu\to {2}\,{\scriptstyle{\bullet} }{\rm{OH}}+{{\rm{O}}}_{2}$$
(2)

The prominent advantages of photocatalytic air purification are (1) no need for chemicals or external energy input except light, which is not costly when utilizing ambient light or sunlight, (2) safe operation under ambient conditions and relatively humidity-insensitive activity, and (3) the ability to fully mineralize volatile organic compounds (VOCs) to CO2 and H2O. On the other hand, this process suffers from low photon utilization efficiency and slow removal rate, difficulty of scaling up, and fouling/deactivation of photocatalysts during prolonged operation.

## Materials and process characteristics in photocatalysis

The best feature of photocatalysis, which distinguishes it from thermal catalysis, is the need for photons, the flux of which limits the overall process. As a result, many PCO reactions are more limited by the photon flux than by the active surface area, unlike most heterogeneous catalysis methods. Photocatalysts absorb photons to generate pairs of electrons and holes that react with dioxygen, water, and surface hydroxyl groups to generate reactive oxygen species (ROS), such as •OH, O2/HO2•, 1O2, and H2O2, which are the key oxidants that decompose air pollutants. As the majority of electron-hole pairs are rapidly recombined, only a tiny fraction of them (less than 1% in many cases) successfully induce PCO reactions. Much effort has been made to improve the photon utilization efficiency for decades, but the successful performance is still limited. The most studied approach is to extend the photocatalyst’s light absorption edge into the visible light range so that more photons can be used3. Analysis of the research literature (published in 1999–2018) on air-purifying photocatalysts shows that modified TiO2 accounts for the largest share (55.9%), followed by Bi-based materials (11.9%) and WO3 (7.3%), among the studied visible-light photocatalysts2. Regarding modified TiO2 materials with visible light activity, most studies have investigated impurity doping and heterojunctions with narrow-bandgap semiconductors or metal nanoparticles. These methods are also useful for increasing the charge separation efficiency and subsequently generating more ROS. It is interesting to note that TiO2-based photocatalysts are still the most studied and the most practical option for air purification applications despite the strong emphasis on the development of new and novel visible light-active materials in academic research. Although modified TiO2 is generally not a strong absorber of visible light, the strong oxidation potential of the TiO2 valence band (VB) edge, along with its excellent stability, low cost and low toxicity, makes it a practical photocatalyst. As a result, a majority of photocatalytic air purification application studies have employed pure and modified TiO2, which does not seem likely to be replaced by new photocatalytic materials in the near future4,5.

The clear trend in photocatalytic material development research is to search for inexpensive and abundant materials with high visible light activity as an alternative to TiO2 to make the technology more feasible. One popular candidate is carbon-based materials such as g-C3N4 and its derivatives, and various carbon nanomaterials such as reduced graphene oxide, carbon nanotubes, and nanodiamond have also been tested to replace costly noble metal cocatalysts (e.g., Pt, Au, Pd)6,7. However, carbon-based materials suffer from low photoactivity and long-term instability under irradiation due to their tendency to be photooxidized. Although more efficient visible light photocatalyst materials have been extensively tested, the redox power of excited electrons and holes in visible light photocatalysts is lower than that of UV-active photocatalysts. Using less energetic photons results in lower redox power; therefore, it should be noted that visible light photocatalysts are not always the best practical solution for air purification purposes.

Another important issue in developing air-cleaning photocatalytic materials is the durability of the materials, which has been far less considered than the photoactivity in most studies, although it is the most critical factor for practical application. It is commonly observed that photocatalysts are gradually deactivated during photoreactions. This can be caused by the intrinsic instability of the photocatalytic material but more often by catalyst surface fouling as a result of the accumulation of recalcitrant intermediates and products. Such catalyst fouling during air treatment is more serious than in the fouling of aqueous-phase photocatalysis, where water as a solvent dissolves the degradation products and intermediates and prevents their surface accumulation. Photocatalyst surface fouling is most often observed during the degradation of aromatic VOCs and heteroatom-containing (e.g., N, S, and P) VOCs as a result of the accumulation of recalcitrant and non-volatile products5,8. In addition, the real-world application of photocatalytic air cleaning should take into account the presence of nuisance components such as dust and aerosol particles that rapidly foul the photocatalyst surface, which seriously limits the outdoor application of this method. Ensuring the long-term durability of photocatalysts in the real world beyond laboratory conditions presents the greatest challenge in commercializing this technology, which has received little attention thus far. The development of practical photocatalytic air purification systems should require a holistic approach that integrates material design/preparation with diverse compositions, structures, and morphology; reaction condition optimization; reactor design and engineering; and hybridization with other technologies (Fig. 1).

Photocatalytic decomposition reactions of various chemical compounds are highly substrate-specific and strongly depend on the molecular structure and composition of target compounds as well as the kind of photocatalyst8,9. There are a wide variety of air pollutants whose photocatalytic removal efficiencies vary greatly, and an enormous number of published studies have reported the photocatalytic degradation of air pollutants. A Google Scholar search for research articles on “photocatalytic degradation of air pollutants” shows 195,000 results! The main problem in analyzing these published results is that it is very difficult to directly compare photocatalytic activity data that were measured with different methods and experimental conditions. Therefore, there is a strong need to standardize the measurements and assessments to compare the photocatalytic activity data reported from different laboratories. To the best of our knowledge, the current air purification ISO methods are only available for the removal of NO, acetaldehyde, toluene, formaldehyde, and methyl mercaptan, but very few studies follow these standards10. More unified and standardized test methods for photocatalytic air purification have yet to be established.

## Some practical considerations for commercial applications

The design, optimization, and scale-up of photocatalytic reactors are challenging issues for the commercialization of photocatalytic air purification. Optimization of the PCO reactor is more complex than that of typical heterogeneous catalytic reactors, as the PCO process should consider both mass transfer and light delivery parameters. An ideal reactor should allow a sufficient number of photons to reach the full surface area of the photocatalyst to maximize the overall air treatment efficiency. The first essential step in preparing practical photocatalytic reactors is to immobilize a durable and robust photocatalyst layer on the support surface. Photocatalysts can be immobilized by various methods, such as the sol-gel technique, thermal spraying, chemical/physical vapor deposition, and electrophoretic deposition, which is usually followed by high temperature roasting to achieve higher crystallinity and stronger adhesion on the support11. This thermal treatment is technically simple but presents a significant hurdle for the practical fabrication of scaled-up reactors because it demands significant energy consumption and a large furnace or heating facilities, which should increase the overall cost. Therefore, the photocatalyst immobilization process without thermal treatment is highly desirable, but remains challenging. The successful development of an ambient-temperature immobilization process will be a breakthrough in facilitating the commercial applications of photocatalysts for various purposes.

For reactor design, plate and annular reactors are usually used in laboratory studies, but they are not suitable as practical reactors because of their low air throughput and reaction area. Monolith-type reactors with a compact structure have high throughput and a low pressure drop, but the light intensity is rapidly extinguished through the monoliths, hindering the uniform illumination of the catalyst surface. To improve the performance of the reactors, upgraded reactors such as multiplate reactors, multiannular reactors, parallel-channel monolith reactors, and radial-leakage optical fiber honeycomb reactors have been developed12.

## Outlook

Using light to clean up polluted air is an ideal technology that mimics nature’s process and has great potential to be developed as a key technology for air purification, which still needs major breakthroughs in several areas. Although current academic research is heavily focused on materials development, engineering for commercialization demands more investigation of practical issues such as preventing photocatalyst fouling/deactivation, facile and low-temperature immobilization of photocatalysts on a support, and effective and economical reactor design. The extensive search for new and novel materials to replace the classic TiO2 material as an air-cleaning photocatalyst has not been very successful for practical purposes, and it is expected that TiO2-based photocatalysts will remain the mainstay material for the time being. Overall, the most suitable application of photocatalytic air purification seems to be indoor air, where pollutants are at the sub-ppm level and interfering substances such as dust and aerosols can be controlled at a minimal level. The ideal scenario for photocatalytic indoor air cleaning is to utilize ambient room light, which requires the development of more active visible-light-responsive materials. Future research on photocatalytic air purification should address practical issues more seriously to bridge the gap between laboratory findings and real-world problems.

## References

1. Vandyck, T. et al. Air quality co-benefits for human health and agriculture counterbalance costs to meet Paris Agreement pledges. Nat. Commun. 9, 4939 (2018).

2. Weon, S., He, F. & Choi, W. Status and challenges in photocatalytic nanotechnology for cleaning air polluted with volatile organic compounds: visible light utilization and catalyst deactivation. Environ. Sci. Nano 6, 3185–3214 (2019).

3. Verbruggen, S. W. TiO2 photocatalysis for the degradation of pollutants in gas phase: From morphological design to plasmonic enhancement. J. Photochem. Photobiol. C 24, 64–82 (2015).

4. Weon, S. et al. Active {001} facet exposed TiO2 nanotubes photocatalyst filter for volatile organic compounds removal: from material development to commercial indoor air cleaner application. Environ. Sci. Technol. 52, 9330–9340 (2018).

5. Weon, S. & Choi, W. TiO2 nanotubes with open channels as deactivation-resistant photocatalyst for the degradation of volatile organic compounds. Environ. Sci. Technol. 50, 2556–2563 (2016).

6. Li, Y. X. et al. Constructing solid-gas-interfacial fenton reaction over alkalinized-C3N4 photocatalyst to achieve apparent quantum yield of 49% at 420 nm. J. Am. Chem. Soc. 138, 13289–13297 (2016).

7. Kim, H. I. et al. Robust co-catalytic performance of nanodiamonds loaded on WO3 for the decomposition of volatile organic compounds under visible light. ACS Catal. 6, 8350–8360 (2016).

8. He, F., Muliane, U., Weon, S. & Choi, W. Substrate-specific mineralization and deactivation behaviors of TiO2 as an air-cleaning photocatalyst. Appl. Catal. B Environ. 275, 119145 (2020).

9. Ryu, J. & Choi, W. Substrate-specific photocatalytic activities of TiO2 and multiactivity test for water treatment application. Environ. Sci. Technol. 42, 294–300 (2008).

10. Zhong, L. X. & Haghighat, F. Photocatalytic air cleaners and materials technologies-Abilities and limitations. Build Environ. 91, 191–203 (2015).

11. Wood, D., Shaw, S., Cawte, T., Shanen, E. & Van Heyst, B. An overview of photocatalyst immobilization methods for air pollution remediation. Chem. Eng. J. 391, 123490 (2020).

12. Ren, H. J., Koshy, P., Chen, W. F., Qi, S. H. & Sorrell, C. C. Photocatalytic materials and technologies for air purification. J. Hazard. Mater. 325, 340–366 (2017).

13. Zou, W. X., Gao, B., Ok, Y. S. & Dong, L. Integrated adsorption and photocatalytic degradation of volatile organic compounds (VOCs) using carbon-based nanocomposites: a critical review. Chemosphere 218, 845–859 (2019).

14. Li, Y. Z., Wu, S. W., Wu, J. C., Hu, Q. Q. & Zhou, C. Y. Photothermocatalysis for efficient abatement of CO and VOCs. J. Mater. Chem. A 8, 8171–8194 (2020).

15. Mohammadi, P., Ghorbani-Shahna, F., Bahrami, A., Rafati, A. A. & Farhadian, M. Plasma-photocatalytic degradation of gaseous toluene using SrTiO3/rGO as an efficient heterojunction for by-products abatement and synergistic effects. J. Photochem. Photobiol. C 394, 112460 (2020).

## Acknowledgements

This work was supported by the Leading Researcher Program (NRF-2020R1A3B2079953) and Korea Research Fellowship Program (Grant No. 2018H1D3A1A02038503), which were funded by the Korea government (MSIT) through the National Research Foundation of Korea (NRF).

## Author information

Authors

### Contributions

F.H., W.J., and W.C. conceived and wrote the manuscript.

### Corresponding author

Correspondence to Wonyong Choi.

## Ethics declarations

### Competing interests

The authors declare no competing interests.

Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.

## Rights and permissions

Reprints and Permissions

He, F., Jeon, W. & Choi, W. Photocatalytic air purification mimicking the self-cleaning process of the atmosphere. Nat Commun 12, 2528 (2021). https://doi.org/10.1038/s41467-021-22839-0

• Accepted:

• Published:

• DOI: https://doi.org/10.1038/s41467-021-22839-0

• ### Design and mechanism of photocatalytic oxidation for the removal of air pollutants: a review

• Kanglu Li
• Hong Wang
• Fan Dong

Environmental Chemistry Letters (2022)

• ### Enhanced photocatalytic performance of Cu2O/TiO2/rGA composites to degrade gas-phase unsymmetrical dimethylhydrazine

• Ruomeng Hou
• Ying Jia
• Nan Jiang

Journal of Materials Science (2022)